High-silica Zeolites as Novel Adsorbents for the Removal of Organic Micro-pollutants in
Water TreatmentJiang, Nan DOI 10.4233/uuid:d4e7d2a8-aed1-48c8-98c3-eb61f18dde0b Publication date 2019 Document Version Final published version Citation (APA)
Jiang, N. (2019). High-silica Zeolites as Novel Adsorbents for the Removal of Organic Micro-pollutants in Water Treatment. https://doi.org/10.4233/uuid:d4e7d2a8-aed1-48c8-98c3-eb61f18dde0b
To cite this publication, please use the final published version (if applicable). Please check the document version above.
Other than for strictly personal use, it is not permitted to download, forward or distribute the text or part of it, without the consent of the author(s) and/or copyright holder(s), unless the work is under an open content license such as Creative Commons. Takedown policy
Please contact us and provide details if you believe this document breaches copyrights. We will remove access to the work immediately and investigate your claim.
This work is downloaded from Delft University of Technology.
Removal of Organic Micro-pollutants
in Water Treatment
Removal of Organic Micro-pollutants
in Water Treatment
For the purpose of obtaining the degree of doctor at Delft University of Technology
by the authority of the Rector Magnificus Prof.dr.ir. T.H.J.J. van der Hagen chair of the Board for Doctorates
to be defended publicly on
Tuesday 10 December 2019 at 10:00 o’clock
Master of Science in Municipal Engineering, Harbin Institute of Technology,
Composition of the doctoral committee:
Rector Magnificus, Chairperson
Prof.dr.ir. L.C. Rietveld Delft University of Technology, promotor
Dr.ir. S.G.J. Heijman Delft University of Technology, promotor
Prof.dr.ir. J.P. van der Hoek Delft University of Technology
Prof.dr.-ing. Habil. T. Wintgens RWTH Aachen, Germany
Prof.dr. M. Yang Chinese Academy of Science, China
Dr.ir. D. de Ridder Evides
Dr. R. Shang Veolia Biothane
Prof.dr.ir. T.J. Heimovaara Delft University of Technology, reserve member
This research study was financed by the Surcharge for Top Consortia for Knowledge and Innovation (TKIs) of the Ministry of Economic Affairs. Nan Jiang acknowledges the China Scholarship Council and Lamminga Fund for providing her scholarship.
Printed by: Gildeprint - the Netherlands ISBN: 978-94-6323-961-5
Copyright © 2019 by Nan Jiang Email: email@example.com
All rights reserved. No part of the material protected by this copyright may be reproduced or utilized in any form or by any means, electronic or mechanical, including photocopying, recording, or by any information storage and retrieval system, without the written permission from the copyright owner.
High-silica zeolites for adsorption of organic
micro-pollutants in water treatment: A review
Adsorption of triclosan, trichlorophenol and
phenol by high-silica zeolites: Adsorption
efficiencies and mechanisms
The adsorption mechanisms of organic
micropollutants on high-silica zeolites
causing S-shaped adsorption isotherms
Adsorption of pharmaceuticals on high-silica
zeolites affected by natural organic matters
Conclusions and outlook
1 The occurrence of organic micro-pollutants
Various pharmaceutically active compounds, pesticides and personal care products, known as organic micro-pollutants (OMPs), are present in drinking water sources and in wastewater treatment plant (WWTP) effluent. Drinking water of impaired quality, contaminated with a high level of OMPs, significantly threatens public health (Kolpin et al., 2002; Pal et al., 2010; Stackelberg et al., 2004). Therefore, the level of OMPs in drinking water is strictly regulated in most countries (Australian Government National Health and Medical Research Council 2011; United States Environmental Protection Agency 2009; World Health Organization 2011). On the other hand, current WWTPs are not designed for OMP removal, giving rise to environmental pollution by OMPs that are discharged to the receiving water body. In response, in some countries, stricter regulations on OMP discharge with the WWTP effluent have been set (Swiss Federal Council 1998).
A range of physical and chemical treatment technologies are found to be effective in reducing the level of OMPs in water, such as membrane filtration, adsorption and (advanced) oxidation (Bal and Dhagat 2001; Klavarioti et al., 2009; Siegrist and Joss 2012). Nanofiltration (NF) and reverse osmosis (RO) membranes reject a large range of OMPs, although the removal of OMPs seems to be incomplete and traces may still be detected in the permeate of NF and RO installations (Verliefde et al., 2007). A drawback of using NF/RO is its high costs and the generation of a waste stream that still contains OMPs. As an alternative, advanced oxidation can efficiently eliminate OMPs in an aqueous environment by inherently changing their structure (Esplugas et al., 2007; Wols and Hofman-Caris 2012). However, the risk of toxic by-product formation arises due to incomplete degradation of OMPs and reactions with other compounds, such as bromide and humic acids in the water (von Gunten 2003b). In contrast, advanced water treatment with activated carbon typically decreases toxic effects (Guzzella et al., 2002; Magdeburg et al., 2014), since compounds are adsorbed onto the material and thus removed from water.
2 Adsorption in drinking water treatment
2.1 Adsorption principles
Adsorption is a phase transfer process that is widely used to remove (organic) substances from fluid phases (Ali and Gupta 2006; Worch 2012). In water treatment, adsorption is defined as the process where solutes, dissolved in water (adsorbates), are removed onto solid surfaces (adsorbents). Adsorption is a dynamic process, where solute adsorption can happen simultaneously with desorption (Figure 1). When the rate of adsorption is equal to the rate of desorption, the system reaches equilibrium. For specific adsorbent and solute, , the equilibrium at constant temperature is determined by:
- Solute concentration in water. In water with single solute, the solute loading on
adsorbents increases with the increase of solute concentration.
- Competing solutes. When competing solutes are present in water, they can
replace the adsorbed solute. The loading of adsorbed solutes on adsorbents will thus decrease (Ruthven 1984).
Figure 1 The adsorption equilibrium in water.
2.2 Applications of activated carbon in water treatment
In drinking water treatment, activated carbon is the most widely used adsorbent to remove undesirable odour, taste, colour, and OMPs. Currently, activated carbon adsorption is applied in all Dutch drinking water treatment plants with surface water sources . Activated carbon can adsorb a broad spectrum of OMPs in water, due to the well-developed pores and high-degree of surface reactivity (Delgado et al., 2012; Mailler et al., 2015). Activated carbon contains pores with a large range of sizes: Micropores, mesopores
and macropores with diameters of < 2 nm, 2 – 50 nm and > 50 nm, respectively. OMPs are mainly adsorbed in the micropores, while mesopores and macropores act as the diffusion routes for OMPs (Ebie et al., 2001). The functional groups and the charges on the carbon surface will affect the affinity of OMPs for activated carbon (Karanfil and Kilduff 1999; Li et al., 2002; Newcombe et al., 1993).
Used activated carbon with toxic residues need to be decomposed or disposed. Saturated activated carbon in granular form can be regenerated off-site by heating. Adsorbed OMPs will decompose and desorb from carbon during regeneration at a temperature of up to 1000 °C (Tipnis and Harriott 1986). Normally, thermal regeneration cause 4 - 10% carbon loss (Hutchins 1973). Powdered activated carbon is also dosed in water to remove OMPs. However, powdered activated carbon cannot be regenerated, leaving undesired toxic residues, which need further treatment before re-entering the environment.
OMP adsorption onto activated carbon can be hampered by the competition with natural organic matter (NOM) in water (Pelekani and Snoeyink 1999; Zietzschmann et al., 2014b). Due to a large variation in pore sizes in the activated carbon, NOM is able to compete with the OMPs which increases the regeneration frequency for activated carbon (Hepplewhite et al., 2004; Newcombe et al., 2002). Besides competition, the relatively large NOM molecules are also known to block pores in the activated carbon. Pore access is thus restricted for solutes and the effective adsorption surface is reduced (Hung et al., 2005; Li et al., 2003a). To avoid their costly regeneration/replacement and the negative effect of
NOM on OMP adsorption, a sound alternative for activated carbon is urgently needed.
3 High-silica zeolites
Zeolites are highly structured porous minerals with pore diameters that are too small for NOM molecules to enter (Auerbach et al., 2003; Baerlocher et al., 2007), thus avoiding the negative influence of NOM that is observed for activated carbon (Hung et al., 2005). Besides, high-silica zeolites have hydrophobic surfaces (Lobo 1997), which could prevent water competition with OMP adsorption from water. Higher adsorption efficiencies of zeolites as compared to activated carbon have been reported for, e.g. methyl tertiary-butyl ether (MTBE) (Abu-Lail et al., 2010; Gonzalez-Olmos et al., 2013; Li et al., 2003b; Rossner and Knappe 2008) and various nitrosamines (de Ridder et al., 2012). Moreover, zeolites
are stable in oxidative conditions, which potentially guarantees the quality and quantity during oxidative regeneration processes (Liu et al., 2014a; Zhang et al., 2014), being a potential for regeneration and operated on-site in the water treatment plant. High-silica zeolites are thus expected to be potential alternative adsorbents for activated carbon in drinking water treatment.
Compared to the studies on activated carbon, only a few studies have been conducted on high-silica zeolites for OMP removal from water. Numerous OMPs with a variety of properties are present in drinking water sources (Luo et al., 2014; Schwarzenbach et al., 2006), while zeolite research has mainly focused on specifically adsorbing OMPs (Anderson 2000; Damjanovic et al., 2010; de Ridder et al., 2012; Rakic et al., 2010; Rossner et al., 2009). There is limited insight in the adsorption mechanisms where zeolites need to adsorb a broad range of OMPs. In addition, more studies are needed for adsorption mechanisms of multi OMPs on specific high-silica zeolites in the presence of NOM.
4 Thesis research framework
Therefore, the objective of this research is to obtain further knowledge on the adsorption mechanisms of high-silica zeolites for a broad spectrum of OMPs, in order to establish an alternative adsorption technology in the current drinking water treatment by the application of high-silica zeolites.
To meet the objective stated above, the following research questions were proposed. The individual research questions were addressed in the chapters of the thesis as listed below:
Research question 1: What is the current understanding of OMP adsorption on high-silica zeolites?
Chapter 2 reflects a literature study focusing on the available knowledge on the
adsorption of OMPs on high-silica zeolites. The physiochemical properties of high-silica zeolites relating to OMP adsorption were introduced. By reviewing the present publications, the already-known OMP adsorption mechanisms on high-silica zeolites was summarized. From there, the feasibility of high-silica zeolites for water treatment was identified, based on the existing knowledge.
Research question 2: What are the OMP adsorption mechanisms on high-silica zeolites?
Chapter 3 describes the adsorption efficacies and mechanisms of OMPs with a variety of
properties on different high-silica zeolites in the batch experiments. The OMP adsorption efficacies were related to the characteristics of OMPs, e.g. molecular sizes and water affinities, as well as the properties of high-silica zeolites, e.g. porous structures and surface properties. On this basis, the dominant adsorption mechanisms were concluded. The featured adsorption mechanisms of high-silica zeolites were highlighted by comparing high-silica zeolites from this study with other commonly used adsorbents, e.g. activated carbon and clays described in literature.
In Chapter 4, a Monte Carlo (MC) simulation is represented to better understand the adsorption mechanisms of OMPs on high-silica zeolites. The main focus was on the occurrence of S-shaped adsorption isotherms, which were firstly observed during OMP adsorption on high-silica zeolites. MC simulation, providing the necessary atomistic resolution, could support the experiments in order to promote a deeper understanding of the governing adsorption mechanisms of OMPs on high-silica zeolites.
Research question 3: How does NOM affect OMP adsorption on high-silica zeolites?
In Chapter 5, the effect of NOM on OMP adsorption on high-silica zeolites is described. The OMP adsorption efficiencies in water without and in the presence of NOM were compared for high-silica zeolites with different porous structures. The effect of OMP characteristics, e.g. hydrophobicity/hydrophilicity, charge and molecular sizes, on the adsorption efficacies of OMPs in the presence of NOM were studied. The mechanisms of NOM affecting OMP adsorption on high-silica zeolites were discussed in this chapter.
HIGH-SILICA ZEOLITES FOR ADSORPTION OF
ORGANIC MICRO-POLLUTANTS IN WATER
TREATMENT: A REVIEW
This chapter is based on: Jiang, N., Shang, R., Heijman, S.G., & Rietveld, L.C. (2018). High-silica zeolites for adsorption of organic micro-pollutants in water treatment: A review. Water research, 144, 145-161.
High-silica zeolites have been found to be effective adsorbents for the removal of organic micro-pollutants (OMPs) from impaired water, including various pharmaceuticals, personal care products, industrial chemicals, etc. In this review, the properties and fundamentals of high-silica zeolites are summarised. Recent research on mechanisms and efficiencies of OMP adsorption by high-silica zeolites are reviewed to assess the potential opportunities and challenges for the application of high-silica zeolites for OMP adsorption in water treatment. It is concluded that the adsorption capacities are well-related to surface hydrophobicity/hydrophilicity and structural features, e.g. micropore volume and pore size of high-silica zeolites, as well as the properties of OMPs. By using high-silica zeolites, the undesired competitive adsorption of background organic matter (NOM) in natural water could potentially be prevented. In addition, oxidative regeneration could be applied on-site to restore the adsorption capacity of zeolites for OMPs and prevent the toxic residues from re-entering the environment.
Organic micro-pollutants (OMPs) have become a worldwide issue of increasing environmental concern (Petrie et al., 2015; Schwarzenbach et al., 2006). In the aquatic environment including drinking water sources and water bodies, OMPs are widely present at trace concentrations ranging from several ng L-1 to a few µg L-1 (Gracia-Lor et al., 2011;
Hughes et al., 2013; Joss et al., 2008). The discharge of OMPs can be attributed to the diffuse sources of pesticides used in agriculture, industrial wastewater effluent, municipal wastewater effluent, etc (Eggen et al., 2014; Gerecke et al., 2002; Lefebvre and Moletta 2006; Michael et al., 2013). The occurrence of OMPs does not only raise toxicological concerns in the aquatic environment (Alan et al., 2008; Santos et al., 2010), but also threatens public health if present in drinking water (Kolpin et al., 2002; Pal et al., 2010; Reemtsma et al., 2016; Stackelberg et al., 2004).
Adsorption of OMPs by porous materials, typically activated carbon, is known as one of the most effective processes for OMP removal and is thus widely deployed (Ahmaruzzaman 2010; Alsbaiee et al., 2016; Stackelberg et al., 2007). Activated carbon adsorbs a broad spectrum of OMPs (Delgado et al., 2012; Karanfil and Kilduff 1999; Rossner et al., 2009;
Snyder et al., 2007) due to the well-developed pore structure, large surface area and high degree of surface reactivity (Dias et al., 2007; Marsh et al., 1997; Moreno-Castilla 2004). However, used adsorbents, with their resultant toxic residues, need to be either decomposed or disposed (Omorogie et al., 2016). To restore the adsorption capacity of used activated carbon and prevent the toxic residues from re-entering the environment, thermal regeneration of activated carbon has been a common practice. During the thermal regeneration process, OMPs that are adsorbed by activated carbon are eliminated by vaporization, pyrolysis and gasification (Sabio et al., 2004; Suzuki et al., 1978; Van Vliet 1991). Nevertheless, the regeneration processes considerably influence the pore structure and chemical functional groups in the activated carbon, which then deteriorates their OMP adsorption performance (Cooney et al., 1983; Martin and Ng 1984). Thermal regeneration of activated carbon could also cause carbon loss of up to 10% in mass (Hutchins 1973; Tipnis and Harriott 1986). New activated carbon has to be purchased and added into the process. Moreover, the OMP adsorption efficiency of activated carbon might be lowered by the co-existence of natural organic matter (NOM) with OMPs, which will reduce the operational period between activated carbon regeneration events (Narbaitz and Cen 1997; Pelekani and Snoeyink 1999; Schork and Fair 1988; Zietzschmann et al., 2014b).
As a feasible alternative, zeolites are crystalline aluminosilicates with orderly distributed and uniformly sized micropores (with a pore diameter less than 2nm) (Li and Yu 2014). Owing to the featured porous properties and chemical composition (Table 1), zeolites can act as molecular sieves and catalysts which are used in the fields of air-pollution remediation, removal of volatile organic compounds, gas separation and catalytic conversion of biomass, etc (Alonso et al., 2017; Ennaert et al., 2016; Li et al., 2017; Perego et al., 2017; Shi et al., 2017; Sun and Wang 2014; Zhang et al., 2016). Based on the unique structural characteristics, framework types of zeolites are defined (refer to Section 2). To date, 235 zeolite frameworks have been assigned at the Structure Commission of the International Zeolite Association (IZA-SC) (Baerlocher and McCusker 2017).
The properties of zeolites vary by the proportion of silica and aluminium content, namely the silica to aluminium ratio (Si/Al ratio). Low-silica zeolites with a Si/Al ratio less than 2 have excellent ion exchange capacity. In the field of water treatment, low-silica zeolites can therefore be applied for softening (Wajima 2012) (Table 1), removal of ammonium (Burgess et al., 2004; Farkas et al., 2005; Kwakye-Awuah et al., 2014), and removal of
heavy metals e.g. zinc (Cerjan Stefanović et al., 2007; Katsou et al., 2010a; Purna Chandra Rao et al., 2006), nickel (Álvarez-Ayuso et al., 2003; Çoruh and Ergun 2009; Katsou et al., 2010b), copper (Ursini et al., 2006) and cadmium (Terbouche et al., 2011).
Table 1. Basic physicochemical properties and the featured application for water treatment of
zeolite and activated carbon.
Zeolite Activated carbon
Porous structure Uniformed micropores a Micropores (< 2 nm), mesopores (2 –
50 nm) and macropores (> 50nm) d
Chemical composition Si, Al, O and cations a C, H, N, S and O d
Surface area 300 – 2300 m2 g-1b 800 – 1500 m2 g-1 d
Featured application for
water treatment Water hardness control ingredients in detergents c
Adsorbents for removal of colour, odour, taste and other undesirable organics in the industrial and
municipal treatment plants d
a (McCusker and Baerlocher 2001)
b Computational Characteristic molecule diameter of 0.6 nm. (First et al., 2011)
c (Maesen and Marcus 2001)
d (Bansal and Goyal 2005)
High-silica zeolites (Figure 1) with Si/Al ratios up to several thousands are industrially manufactured by replacing the aluminium contents with silica (Burton 2018; Burton et al., 2005). The hydrophobicity of these zeolites provides favourable characteristics for OMP adsorption in aqueous solutions (Maesen 2007; Tsitsishvili 1973). Currently, high-silica zeolite powders have been proven to be effective adsorbents for the removal of OMPs from water, including pharmaceuticals, personal care products and industrial chemicals, based on information provided only by batch tests (Damjanovic et al., 2010; Rakic et al., 2010; Rossner et al., 2009). However, the application of high-silica zeolite granules in full-scale water treatment has not been realized yet.
Figure 1. Commercial high-silica zeolite (a) powders; (b) granules with cylindrical and spherical
As a type of aluminosilicate crystal, zeolites are stable in oxidative conditions, which potentially guarantees the regeneration of zeolites by (advanced) oxidation without compromising their surface properties and pore structure (Liu et al., 2014a; Zhang et al., 2014). Combining zeolite adsorption and oxidation regeneration can restore the adsorption capacity of zeolites in situ and degrade or mineralize OMPs (Zhang et al., 2014). Concentrated toxic residues from the adsorption process will be thus minimized by oxidation. Therefore, effective oxidative regeneration of zeolites without impairing the quality and quantity of adsorbents could be a key advantage over activated carbon as a benchmark technology.
In this review, the literature on high-silica zeolites for OMP adsorption from water is reviewed, including the fundamentals of the zeolite frameworks, the physicochemical properties and their relation to OMP adsorption. The adsorption mechanisms of high-silica zeolite powders are elaborated by considering the properties of zeolites and variety of OMPs. Examples of the application of high-silica zeolite granules are presented. Finally, the potential opportunities and challenges of applying high-silica zeolites to water treatment are discussed.
2. Physicochemical properties of high-silica zeolites
Zeolites have a 3-dimensional structure constructed by TO4 tetrahedra, where the T atom
is either a Si4+ or Al3+ atom located in the centre of an oxygen tetrahedron. Since each Al3+
atom introduces one negative charge, the same number of cations can associate loosely with the tetrahedral-coordinated Al3+ to neutralize the entire framework. The ratio of Si4+
and Al3+ in the framework, known as the silica-to-alumina ratio, is commonly written as
either SiO2/Al2O3 mole ratio or Si/Al mole ratio by different authors. In this review, the
Si/Al ratio is used to describe the hydrophobicity of zeolite surface, which is two times of the SiO2/Al2O3 mole ratio (McCusker and Baerlocher 2001).
The framework of zeolites describes the connectivity of the tetrahedrally coordinated atoms (T-atoms) without reference to elemental composition. The framework type exclusively defines the structural properties of zeolites including pore opening, cage and channel structure (McCusker and Baerlocher 2001).
• The pore opening of zeolites, composed by T atoms and the connected oxygen
atoms, is the entry of a cage or a channel which will decide the entering of OMPs. The pores with more T atoms/oxygen atoms have larger sizes. The pore opening could be described as an n-ring, e.g. 8-, 10-, and 12-rings, where n represents the number of T or oxygen atoms.
(a) (b) (c) (d)
Figure 2. Examples of pore opening of zeolites (Baerlocher et al., 2007). (a) 12-ring opening in
FAU zeolites, (b) 8-ring & 12-ring opening in MOR zeolites, (c) 12-ring opening in BEA zeolites, (d) 10-ring opening in MFI zeolites (framework type codes of the zeolites, referring to Table 2).
• The pore space of zeolites is parcelled into cages and/or channels. Cages, also
called cavities, are the polyhedral units in zeolites, while channels in zeolites are composed by linked polyhedral units. The channels of zeolites vary from straight to sinusoidal forms or from wide to narrow. Many adsorption-related properties of zeolites, e.g. surface area and pore volume, are decided by the features of the cages and channels.
Figure 3. Examples of cages and channels of zeolites (a) Schematic representation showing cages
in FAU type zeolites (Baerlocher et al., 2007), (b) ‘hollow-tube’ representation showing channels in MFI zeolites (Rhodes 2010) (FAU and MFI are framework type codes of the zeolites, referring to Table 2)
Table 2. Key properties of four commonly used frameworks of zeolites.
Framework Ring number and pore opening size a Framework density a Accessible
(m2 g-1) b
Maximum diameter of a sphere b
Type Structure a Å×Å Å×Å T atoms
(Å3)-1 can be included (Å) can diffuse along (Å*Å*Å) FAU 12 ring 7.4×7.4 12.7 1211.42 11.24 7.35*7.35*7.35
MOR 12 ring 6.5×7.4 8 ring 2.6×5.7 17.2 1010.22 6.70 1.57*2.95*6.45
BEA 12 ring 6.6×6.7 12 ring 5.6×5.6 15.1 1220.45 6.68 5.95*5.95*5.95
MFI 10 ring 5.1×5.5 10 ring 5.3×5.6 17.9 834.41 6.36 4.70*4.46*4.46
a (Baerlocher et al., 2007)
b The accessible area is the area of that surface visited by the centre of the water molecule in the idealised
framework model. Accessible area and maximum diameter of a sphere were calculated by Mike Treacy, Arizona State University, using his codes "TOTOPOL" and "DelaneysDonkey." (Foster et al., 2006).
The structural features of high-silica zeolites are mostly determined by their framework types. A framework type represents a unique structure of channels and cages that will highly affect the adsorption efficiency of OMPs. FAU, MOR, MFI and BEA types of high-silica zeolites were selected for review, because they are the most commercially available and have been commonly studied for OMP adsorption. Their structural features are summarized in Table 2.
All selected framework types contain a high accessible area (from 834 to 1220 m2 g-1 in
Table 2) for the adsorption of both water and organic compounds. The framework density
is related to the pore volume such that zeolites with a lower framework density have a higher pore volume (Meier and Baerlocher 1999). The pore volume of zeolites would follow the opposite order of framework density, namely FAU > BEA > MOR > MFI (Table 2). The effect of pore volume on OMP adsorption will be discussed in section 3.1.
The properties of high-silica zeolites with the same framework type and Si/Al ratio vary. Theoretically, ideally crystalized zeolites with the same framework type and Si/Al ratio show identical properties. However, high-silica zeolites are synthesised from low-silica zeolites by dealuminating, which would bring defects to the framework (Yu et al., 2007). Therefore, the micropore volume of high-silica zeolites with the same framework types could vary (Yonli et al., 2012). Their actual surface area is usually less than what would be found in the ideal framework (Dubinin 1967). In addition, mesopores in zeolites, generated during the dealumination process, account for a small portion of the entire surface area of zeolites, mainly as external surface area (Yonli et al., 2012). As a result, the adsorption efficiency of the “same type” high-silica zeolites is similar but to some extent different due to the variation in properties.
3. Adsorption mechanisms and factors affecting the adsorption of
OMPs by high-silica zeolite powders
In aqueous solutions, the overall adsorption efficiency of OMPs by high-silica zeolite powders is represented in Equation 2-1 (Israelachvili 2015):
where Wij is the work to separate two phases, i and j, and the subscripts z, o and w refer to
zeolite, OMP and water, respectively. Wozw is the work of adhesion of the OMP to zeolites in
water, e.g. the adsorption energy of the OMP by the zeolite in aqueous solution, which will
decide the adsorption efficiency. Water cohesion (Www) describes the interaction between
water molecules. In the discussion, water cohesion is regarded as a constant parameter with negligible effect on adsorption efficiency. The OMP adsorption efficiency by high-silica zeolites will depend on the OMP-zeolite interaction (WOZ), zeolite-water interactions,
(WZW) and OMP-water interactions (WOW), which will include the effect of structural
features, surface hydrophobicity and existing adsorption sites of high-silica zeolites as well as characteristics of OMPs.
3.1 Structural features and framework types of high-silica zeolitesThe adsorption of OMPs primarily takes place in the micropores of the high-silica zeolites. In many studies, the adsorption saturations were observed and the isotherms were fitted by the Langmuir model (Table 4), which indicate the occurrence of monolayer adsorption in micropores (Sing 1985). In some cases, mesopores could still provide additional accommodation for OMPs (Martucci et al., 2012). For example, when adsorption takes
place in the presence of high concentrations of organic solutions (g L-1), a strong
adsorption driving force at the high equilibrium concentration may lead to pore filling in the mesopores, which will increase the adsorption capacity. During the pore filling process, both adsorption and absorption may occur (Damjanovic et al., 2010).
The adsorption capacity of zeolites can thus be well-correlated to their microporous volume. Several studies found that FAU and BEA zeolites with larger micropore volumes showed a higher adsorption capacity for OMPs (Koubaissy et al., 2012; Reungoat et al., 2007; Yonli et al., 2012). As an example, FAU zeolite was found to have a higher adsorption capacity for nitrobenzene than BEA, MFI and MOR type zeolites (Reungoat et al., 2007). Compared to MFI type zeolites, BEA also has a higher adsorption capacity for phenol, dichlorophenol and nitrobenzene since the BEA type framework possesses a higher micropore volume (Damjanovic et al., 2010; Koubaissy et al., 2008; Reungoat et al., 2007). The pore opening size of zeolites determines the diffusivity and accessibility of the OMPs during the adsorption process. OMPs with a molecular size smaller than the pore opening size of zeolites can easily diffuse inside zeolite powders due to negligible steric hindrance
(Roque-Malherbe et al., 1995; Rungsirisakun et al., 2006). Certain OMP molecules, e.g. carbamazepine, may form molecular chains of enlarged size due to the molecular interactions. The molecular chain of carbamazepine could enter the FAU zeolite, which has a large pore opening size, but could not enter the MOR and MFI zeolites, which have
narrow channel openings (Martucci et al., 2012).The adsorption of OMPs is minimal when
the size of OMPs are larger than the pore opening size of zeolites. Zeolites would then behave as molecular sieves, resulting in the exclusion of OMPs from the framework of zeolites (Rouquerol et al., 2013).
Multiple studies showed that OMPs with environmentally relevant concentrations, ranging from ng L-1 to µg L-1, were preferably adsorbed by high-silica zeolites with pore sizes
closely similar to the molecular size of OMPs, so-called close-fit theory (de Ridder et al., 2012; Rossner et al., 2009). A common explanation is that the closely fitted pores may lead to strong interactions between OMPs and high-silica zeolites (de Ridder et al., 2012; Erdem-Senatalar et al., 2004; Rossner et al., 2009). Giaya and Thompson (2002a; 2002b) also suggested that the structure of water clusters might be disrupted in the well-fitted pores, which would promote the affinities for OMPs. For example, all seven tested
N-nitrosamine compounds (MW: 74 – 158 g mol-1, estimated stokes diameter 2.6 - 4.0 Å) with
an initial concentration of 15 µg L-1 could not be removed by FAU zeolites, while MOR and
MFI with small pore sizes (see Table 2) removed five N-nitrosamines from the seven tested compounds. MOR and MFI zeolites, possessing comparable pore opening and channel sizes as N-nitrosamine compounds, were thus suitable for their removal at these low concentration ranges (de Ridder et al., 2012). In another study, Rossner et al. (2009)
compared the removal of 25 emerging OMPs (MW: 151 - 791 g mol-1, estimated spherical
diameter: 6.5 – 9.5 Å) from lake water with initial concentrations less than 1 µg L-1 by MFI,
MOR and FAU zeolites. A total of 15 OMPs were either partially or completely removed by MOR zeolites, while FAU could only remove 3 OMPs to an acceptable level. Two types of zeolites with relatively small pore openings, MFI zeolites with 10-ring pores and MOR zeolites with 12- & 8-ring pores, were proven to be effective for the adsorption of these low molecular weight OMPs at low concentrations. It was found that the molecular size of these OMPs was similar to the pore opening size or channel size of MFI and MOR zeolites.
3.2 Surface hydrophobicity and Si/Al ratio of high-silica zeolites
Surface hydrophobicity is defined as the absence of ‘strong sorption’ of polar compounds, particularly water (Olson et al., 2000). Highly hydrophobic zeolites could prevent water uptake (Damjanovic et al., 2010; de Ridder et al., 2012). Thus, the pore blockage by water clusters could be inhibited, resulting in more pores of zeolites available for OMP diffusion and adsorption (de Ridder et al., 2012; Guvenc and Ahunbay 2012).
The chemical composition of zeolites strongly influences the hydrophobicity and zeolite-water interaction. Bolis et al., (2006) proposed that zeolite-water molecules can interact with Al sites of zeolite framework. In addition, the hydrophobicity can be influenced by a small number of Si-OH species, which are located at the defects in the zeolites, since Si-OH species could adsorb water by forming stable adducts.
For zeolites with the same framework type, the hydrophobicity increases with decreasing aluminium content, thus zeolites with higher Si/Al ratios are more hydrophobic(Chen 1976; Eberly Jr et al., 1971; Nakamoto and Takahashi 1982; Olson et al., 1980). It can be concluded that zeolites with higher Si/Al ratios (examples found in Table 3) exhibit a higher adsorption capacity than the zeolites of the same framework with a low Si/Al ratio (Anderson 2000; Damjanovic et al., 2010; Grieco and Ramarao 2013; Li et al., 2003b; Reungoat et al., 2007; Yonli et al., 2012). In the case of α-endosulfan and tris-2-chloroethyl phosphate adsorption, the zeolites with a higher Si/Al ratio, regardless of their slightly lower surface area, have a higher adsorption capacity for OMPs (Table 3). The adsorption of nicotine using zeolites, however, is an exception. Rakic et al., (2010) reported a higher adsorption capacity of nicotine on BEA zeolite with a lower Si/Al ratio. The results were driven by specific adsorption site interactions, which will be further explored in section 3.4. When the Si/Al ratio is high enough, the hydrophobicity of zeolites is no longer of significant importance because the effect of water competition and water cluster hindering has become negligible. Gonzalez-Olmos et al., (2013) found that by increasing the Si/Al ratio from 800 to 1366, MFI zeolites did not improve their adsorption capacity of MTBE, and even a slight decrease was observed when the surface area of zeolites increased from 265 to 330 m2 g-1. In addition, the adsorption capacities for 4-chlorophenol increased by 28%
when the Si/Al ratio increased from 504 to 2252, but there was little effect after further increase in the Si/Al ratio (Shu et al., 1997). For nitrobenzene, the adsorption capacity of
BEA and MFI zeolites were also related to its Si/Al ratio for those with a low Si/Al ratio. However, the adsorption capacity of zeolites became independent of the Si/Al ratio for ratios over 800 in this case (Reungoat et al., 2007).
Table 3. The maximum adsorption capacities from the Langmuir isotherm by adjustment to the
properties of zeolites for the adsorption of OMPs on high-silica zeolites.
Adsorbate QL (mg g-1)a Si/Al ratio BET surface
area (m2 g-1) C0 (mg L-1)b Framework type of zeolite Reference Nitrobenzene 75.6 84 531 600 BEA (Reungoat et al., 2007) 95.0 196 700 600 BEA 83.9 80 300 600 MFI 118.7 200 300 600 MFI 147.6 800 300 600 MFI 135.7 1800 300 600 MFI α-endosulfan 500.0 43 789 10-30 FAU (Yonli et al., 2012) 666.6 51 830 10-30 FAU 833.3 68 825 10-30 FAU 763.4 72 546 10-30 BEA 787.4 126 594 10-30 BEA 793.7 220 528 10-30 BEA Phenol 28.2 30 392 ~2820 MFI (Damjanovic et al., 2010) 31.0 80 425 ~2820 MFI 38.5 280 400 ~2820 MFI Tris-2-chloroethyl phosphate
76.6 50 680 10 BEA (Grieco and
Ramarao 2013) 103,0 600 620 10 BEA Methyl tert-butyl ether 6.5 472 385 1-100 MFI (Gonzalez-Olmos et al., 2013) 15.2 800 265 1-100 MFI 14.1 1366 330 1-100 MFI
Nicotine 240 50 741 4.9 BEA (Rakic et al., 2010)
60 172 650 4.9 BEA
a QL is the maximum adsorption capacity of high-silica zeolites estimated from Langmuir isotherm.
Since the hydrophobicity of high-silica zeolites is well-related to Al content, the adsorption capacity could be strongly-correlated to the Al content (Al%) (Khalid et al., 2004), which can be expressed by:
Al% =𝑆𝑆𝑆𝑆+𝐴𝐴𝐴𝐴𝐴𝐴𝐴𝐴 ∗ 100% =1+𝑆𝑆𝑆𝑆 𝐴𝐴𝐴𝐴⁄ 𝑟𝑟𝑟𝑟𝑟𝑟𝑆𝑆𝑜𝑜1 ∗ 100% Equation 2
For high-silica zeolites with the same framework, Al% of high-silica zeolites has a negative linear correlation with the adsorption capacity of various OMPs (Figure 4). Therefore, Al% may serve as an indicator of adsorption capacity in the high Si/Al ratio range.
Figure 4. The effect of Al% for the adsorption capacity of various OMPs. Data source: nitrobenzene
(Reungoat et al., 2007), MTBE (Gonzalez-Olmos et al., 2013), alpha-endosulfan (Yonli et al., 2012) and phenol (Damjanovic et al., 2010)
In place of Si/Al ratio and Al content, hydrophobicity index (HI) was applied to represent hydrophobicity of zeolites by Yonli et al., (2012). The value of HI could be determined by: HI = 𝑋𝑋𝑡𝑡𝑡𝑡𝑡𝑡𝑡𝑡𝑡𝑡𝑡𝑡𝑡𝑡
𝑋𝑋𝑤𝑤𝑤𝑤𝑡𝑡𝑡𝑡𝑤𝑤 Equation 3
where Xtoluene represents toluene adsorption capacity (g g-1) and Xwater represents water
adsorption capacity (g g-1). For the FAU and BEA zeolites, there was a linear increase of
α-endosulfan adsorption efficiency with the increase of HI.
0.0 0.5 1.0 1.5 2.0 2.5 0 100 200 300 400 500 600 700 800 900 Nitrobenzene - MFI MTBE - MFI Alpha-endosulfan - FAU Alpha-endosulfan - BEA Phenol - MFI qe (mg g -1 ) Al%
The increased adsorption efficiency of OMPs by high-silica zeolites with the same framework could thus be related to the hydrophobicity of high-silica zeolites, which, in its turn, could be predicted by Si/Al ratio, Al content and HI index. However, the hydrophobicity of zeolites with different framework types should not be compared only by reference to Si/Al ratio but also by the structural features of the zeolites. For example, MFI zeolites are more hydrophobic than FAU zeolites with the same Si/Al of 80 because the smaller confinement pore space of MFI zeolites disrupts the interactions of water molecules such that water can hardly stay inside the pores (Damjanovic et al., 2010; de Ridder et al., 2012; Giaya and Thompson 2002b). In this case, the adsorption efficiency of OMPs by high-silica zeolites is then better determined by framework type.
3.3 Characteristics of OMPs
The effects of surface charge and the ionization form of the OMPs on the adsorption efficiency of high-silica zeolites have been studied (Bautista-Toledo et al., 2005; Janos et al., 2003). High-silica zeolites have a limited number of cations and negative charges around Al sites, while most of the framework structures remain neutral (no ionized sites). The preferential adsorption of neutral OMP species by high-silica zeolites was observed (Fukahori et al., 2011; Grieco and Ramarao 2013; Koubaissy et al., 2012; Simon et al., 2015; Tsai et al., 2006). For example, the neutral aromatic compounds, e.g. nitroaniline and chlorophenol, were preferentially adsorbed onto FAU zeolite compared to the ionic compounds (Koubaissy et al., 2011). Fukahori et al., (2011) reported that sulfa drugs in neutral form could be more readily adsorbed onto FAU zeolites than those in cationic and anionic forms, based on the hydrophobic interactions.
When OMPs in anionic forms are dominant under alkaline conditions, a reduction of adsorption capacity has been observed (Chen et al., 2015; Koubaissy et al., 2011). Since high-silica zeolites employ a large amount of electron-rich oxygen sites and very few negative sites, repulsion forces between the anionic form of the OMPs and the zeolite surface arise (Fukahori et al., 2011; Koubaissy et al., 2011; Koubaissy et al., 2012). The removal mechanism of cationic OMPs by adsorbents has been regarded as ion exchange. As high-silica zeolites possess few exchangeable ions, the removal capacity of cationic OMPs by high-silica zeolites might be less than that of the low-silica zeolites, e.g. natural zeolites (Margeta et al., 2013). Since the ionization of OMPs is affected by the relationship between
pH value in an aqueous solution and the pKa value of OMPs, the pH of the solution should
therefore be taken into consideration in the adsorption process.
Previous studies have shown that the decreased interactions between OMP and water will enhance OMP-zeolite interaction, and a strong correlation between the adsorption capacity and hydrophobicity of OMPs has been observed (Fukahori et al., 2011; Koubaissy et al., 2011; Koubaissy et al., 2008). It was found that hydrophilic N-Nitrosodimethylamine (NDMA) and N-Nitrosomethylethylamine (NEMA) were not adsorbed by MFI nor MOR zeolites, while less hydrophilic N-nitrosamines with comparable sizes to NDMA and NEMA were adsorbed to a larger extent (de Ridder et al., 2012). Similar results were reported by Zhu et al., (2001). The interaction between neutral OMP molecules and water can be
described by the octanol-water coefficient (Kow). When the effect of OMP charge is
considered, the interaction could be expressed by the distribution coefficient, logD, which
is calculated from Kow, pKa of OMPs and pH of the aqueous solution. Neglecting the
interaction between OMPs and octanol, OMPs with higher Kow and logD are more
hydrophobic and less soluble in water (Gschwend 2016).
3.4 Adsorption forces and possible adsorption sites of high-silica zeolites
Much effort has been dedicated to determining adsorption forces and locations of adsorbed OMPs, which would give further insight into how high-silica zeolites interact with OMPs. The adsorption of OMPs by high-silica zeolites is a physical process attributed mainly to Van der Waals forces (Blasioli et al., 2014). Aside from the Van der Waals forces, acid-base forces exist between the functional groups of OMPs and the specific sites of
zeolites, so-called “adsorption sites.” Theheterogeneity of the adsorption sites has been
indicated from the results of adsorption heats during OMP adsorption by high-silica zeolites (Damjanovic et al., 2010; Rakic et al., 2010). From simulation results of a Monte Carlo study and Rietveld’s analysis, MFI and FER zeolites were proved to employ different types of sites for OMPs adsorption (DeJaco et al., 2016).
Two typical adsorption sites of high-silica zeolites, oxygen and acidic sites, have been identified in literature. Oxygen atoms in the framework of zeolites widely exist as oxygen sites. OMPs with hydrogen on the aromatic ring and amino groups show an acidic character and have an affinity for oxygen sites (Blasioli et al., 2014; Koubaissy et al., 2011).
The results of Blasioli et al. (2014) indicate that sulfamethoxazole interacts with FAU and MOR zeolites by weak H-bonds.
A limited number of Brønsted and Lewis acidic sites in high-silica zeolites are known to interact with OMPs with nucleophilic groups, e.g. sulphur or chlorine atoms (Bolis et al., 2006; Damjanovic et al., 2010; Nikolakis 2005; Phung and Busca 2015). The specific interaction may lead to chemisorption and higher adsorption energy (Batonneau-Gener et al., 2010). Acidic sites may thus promote the adsorption of certain OMPs on high-silica zeolites. Rakic et al., (2010) reported a higher adsorption capacity of nicotine on BEA zeolite with a lower Si/Al ratio and more acidic sites. Nicotine is an organic base with basic nitrogen atoms acting as an amine (de Lucas et al., 1998). The adsorption mechanism could be explained by the neutralisation of nicotine by the acidic sites on the zeolites.
4. Potential applications of high-silica zeolites for water treatment
4.1 Adsorption of OMPs by high-silica zeolites
The efficiency of high-silica zeolites for OMP adsorption and their isotherm fitting constants are summarised in Table 4. Results are collected from batch-scale experiments applying high-silica zeolite powders.
In this section, we first discuss the adsorption of specific OMPs, including MTBE, nitrosamines, phenol and phenolic compounds, which were studied at high equilibrium
concentrations, e.g. mg L-1. Afterwards, OMP adsorption at environmentally relevant
concentrations, e.g. ng L-1 and µg L-1, is discussed in the sub-sections “OMP mixtures” and
“Prediction of adsorption on high-silica zeolites at environmentally relevant concentrations”. A few studies on the application of high-silica zeolite granules in column-scale experiments will be discussed at the end of this section.
Methyl tertiary-butyl ether (MTBE) is a widely used fuel additive with a good aqueous
solubility, 51,000 mg L-1 at 25 °C. MTBE is frequently found in surface water and
groundwater (Achten et al., 2002; Squillace et al., 1996). Various types of zeolites can adsorb MTBE from water, e.g. BEA, MFI and MOR zeolites (Knappe and Campos 2005; Li et
al., 2003b). At the equilibrium concentration of 1 mg L-1, MOR zeolites with a Si/Al ratio of 180 exhibited an adsorption capacity of 22 mg g-1, while the capacity of carbonaceous resins and activated carbon were 15.6 mg g-1 and 14.0 mg g-1, respectively (Davis and Powers 2000; Erdem-Senatalar et al., 2004; Melin 1999). BEA zeolites had a capacity of 8 mg g-1, and MTBE adsorption was negligible on the FAU at the equilibrium concentration of 1 mg L-1 since the pore opening and cage size were much larger than the size of MTBE (Erdem-Senatalar et al., 2004). High-silica zeolites with closely fitted pores for MTBE, e.g. MFI and MOR types, are more effective adsorbents for MTBE removal than BEA and FAU
zeolites at the equilibrium concentration range 0.1 – 1000 µg L-1 (Knappe and Campos
Nitrosamines are a group of disinfection by-products with a molecular weight less than
200 g mol-1. Most of them are classified as probable human carcinogens and have been
detected in both water sources and drinking water (Mitch et al., 2003; Zhao et al., 2008). At
initial concentrations of 5mg L-1, the NDMA adsorption capacity of MFI zeolites was 0.196
mg g-1, which was 4 – 7 times greater than the tested FAU and MOR zeolites (He and Cheng
2016). MFI and MOR zeolites were able to adsorb five species of N-nitrosamines, namely N-Nitrosomorpholine (NMOR), N-Nitrosopiperidine (NPIP), N-Nitrosodiethylamine (NDEA), N-Nitrosodi-n-propylamine (NDPA) and N,N-Dibutylnitrosamine (NDBA) at an
initial concentration of 15 µg L-1, while activated carbon showed a lower nitrosamine
removal (de Ridder et al., 2012). Zhu et al. (2001) reported that MFI zeolites had an adsorption capacity of 9.2 mg g-1 for NDMA and 16.7 mg g-1 for N-nitrosopyrrolidine (NPYR)
at the equilibrium concentration ~ 480 mg L-1, which was also higher than the capacity of
FAU zeolites. To minimize the formation of N-nitrosamines, high silica zeolites could also be applied to remove the secondary and tertiary amines, which are nitrosamines formation precursors. More than 90% of the nitrosamines’ precursors could be removed
by MOR zeolites when the dosage of zeolites was 100 mg L-1 in laboratory reagent water.
To remove N-nitrosamine precursors, MOR zeolites were reported to be more effective than the tested activated carbon (Wu et al., 2015).
Different types of zeolites were applied for adsorption of phenol and phenolic compounds. Khalid et al. (2004) demonstrated that pure silica BEA zeolite (no Al content) employed the best performance among all tested zeolites, i.e. MOR, BEA and FAU zeolites as well as activated carbons at a phenol equilibrium concentration <1.6 g L-1. The FAU zeolites had the fastest kinetics for phenol adsorption among other studied adsorbents: activated carbon, activated alumina and silica gel (Roostaei and Tezel 2004). From the experimental results of the nitrophenolic compounds’ adsorption, FAU type zeolites and pure silica BEA zeolites possessed a much higher capacity than MFI. The highest capacity for nitrophenolic compounds (ortho-nitrophenol) was 240 mg g-1 at an equilibrium concentration of 50 mg L-1, achieved by FAU zeolites (Koubaissy et al., 2008). However, Zhang et al. (2014) studied the adsorption of 2,4,6-trichlorophenol (TCP) by FAU zeolites and found that the adsorption capacity reached 3.06 mg g-1 at an equilibrium concentration of 30 mg L-1, much less than the capacity of granular activated carbon with a capacity of ~500 mg g-1 (Nelson and Yang 1995).
Ta bl e 4 . T he a pp lic at io n o f h ig h-sil ic a z eo lit es fo r O M P a ds or pt io n, th e is ot her m in fo rm at io n a nd ex per im en ta l c on dit io ns . Ad so rb at e Fra mew ork ty pe o f ze ol ite (S i/ Al rat io ) Is ot he rm ty pe Is ot he rm co ns ta nt s Fr eu nd lic h is oth er m f itti ng co ns ta nt s * Ex pe ri m ent al co nd iti ons KF (µg g -1)( L µg -1) n n M et hy l te rt -bu ty l e th er (M TBE ) M FI (1 36 6) Fr eu nd lic h K F (m g kg -1)( L mg -1) n 43 70 0 n 0.95 - 61 .7 3 0. 95 1-2 g z eo lite s w er e d os ed in MT BE sol ut ion w ith co nce nt ra tio n 1 -1 00 m g L -1 Th e fit te d c on ce nt ra tio n ran ge f or M FI z eo lit es w as 0. 01 – 0 .7 9m g L -1 an d 0 .0 1-32 m g L -1 fo r BE A a nd F AU ze ol ite s. M FI (8 00 ) Fr eu nd lic h K F (m g kg -1)( L mg -1) n 43 40 0 n 0.88 - 99 .4 3 0. 88 M FI (4 72 ) Fr eu nd lic h K F (m g kg -1)( L mg -1) n 11 30 0 n 1.07 - 6. 97 1. 07 BE A( 40 0) Fr eu nd lic h KF (m g kg -1)( L mg -1) n 24 30 n 0.98 - 2. 79 0. 98 FA U( 40 0) Fr eu nd lic h KF (m g kg -1)( L mg -1) n 36 3 n 1.15 - 0. 13 1. 15 N -N itr os od imet hy la mi ne (N DMA ) FA U( 40 ) Fr eu nd lic h KF (nm ol g -1)( L n mo l -1) n 0. 01 79 n 0.87 - 0. 07 0. 87 Ze ol ite s (~ 10 0 m g) w er ad de d in to 40 m L gla ss v ia ls con ta in in g 30 m L of N DM A so lu tio ns at va ry in co nce nt ra tio ns ( 1 8 - 7 40 µ L -1). M FI (1 2. 5) Fr eu nd lic h KF (nm ol g -1)( L n mo l -1) n 0. 17 34 n 1.03 - 0. 12 1. 03 M FI (2 5) Fr eu nd lic h KF (n m ol g -1)( L nm ol -1) n 0. 11 19 n 0.92 - 0. 25 0. 92 M FI (4 0) Fr eu nd lic h KF (nm ol g -1)( L n mo l -1) n 0. 45 88 n 0.95 - 0. 80 0. 95 M FI (1 30 ) Fr eu nd lic h K F (nm ol g -1)( L n mo l -1) n 0. 44 47 n 0.89 - 1. 40 0. 89 N -N itr os om or ph ol in e (N MO R) M FI (8 0) Fr eu nd lic h K F (µg g -1)( L µ g -1) n 17 n 1.04 - 17 1. 04 Th e in iti al co nce nt ra tio n o eac h of t he n itr os am in es 25 | Li te ra tu re re vi ew
26 | Cha pte r 2 N -N itr os om or ph ol in e (N MO R) MO R(2 00 ) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 2 n 1.70 - 2 1. 70 w as 1 5 µ g L -1. T he ad so rb en t co nc en tr ati on va ried b etw ee n 1 0 an d 20 0 m g L -1. N -N itr os op ip er id in e (N PI P) M FI (8 0) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 49 1 n 1.11 - 49 1 1. 11 N -N itr os op ip er id in e (N PI P) MO R(2 00 ) Fr eu nd lic h K F (µg g -1)( L µ g -1) n 18 7 n 0.99 - 18 7 0. 99 N -N itr os od ie th yl am in e (N DE A) M FI (8 0) Fr eu nd lic h K F (µg g -1)( L µ g -1) n 30 3 n 1.65 - 30 3 1. 65 N -N itr os od ie th yl am in e (N DE A) MO R(2 00 ) Fr eu nd lic h K F (µg g -1)( L µ g -1) n 43 n 0.65 - 43 0. 65 N -N itr os od i-n -pro py la m in e ( N DP A) M FI (8 0) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 9. 04 ×1 0 4 n 1.20 - 9. 04 *1 0 4 1. 20 N -N itr os od i-n -pro py la m in e ( N DP A) MO R(2 00 ) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 15 74 n 0.91 - 15 74 0. 91 Ph eno l BE A( 43 ) Si ps Qs (m ol g -1) 0. 00 06 4 Ks(L m ol -1) βs 76 6. 99 βs 1.20 0. 01 2 1. 20 10 0 mg d ry z eo lit e w as do sed in 1 .5 ml w at er w ith an a pp ro pri at e a m ou nt o f 0. 03 m ol L -1 ph eno l so lu tio n. T he eq ui libr iu m co nce nt ra tio ns a t 30 3K w er e ac hi ev ed a fte r 1h o f st ir ri ng . M FI (1 5) Si ps Qs (m ol g -1) 0. 00 03 Ks(L m ol -1) βs 26 .3 βs 0.66 4. 03 0. 65 M FI (4 0) Si ps Qs (m ol g -1) 0. 00 03 3 Ks(L m ol -1) βs 71 1. 53 βs 0.94 0. 71 0. 93 M FI (1 40 ) Si ps Qs (m ol g -1) 0. 00 04 1 Ks(L m ol -1) βs 59 63 4. 37 βs 1.73 3. 70 *E -5 1. 73 Bi sp he no l-A MO R(1 80 ) Re dl ic h-pe te rs on K R (L m g -1) 0. 73 5 a R (L m g -1) β 1. 0 β R 0.59 19 27 5. 24 0. 23 0. 5g L -1 dr y z eo lit e w as do se d i n bi sp hen ol -A so lu tio n w ith co nce nt ra tio n 10 -3 0 m g L -1. Tr ich lo ro ph en ol FA U( 60 ) Fr eu nd lic h KF (m g g -1)( L m g -1) n 1. 80 *1 0 -3 n 0.43 - 0. 09 0. 43 1 g o f z eo lit e w as a dd ed to 50 m L o f TC P so lu tio n w ith dei on is ed w at er a t d iff er en t co nc en tr at io ns ( 10 , 2 5, 5 0,
75 , a nd 1 00 m g L -1). 2-ni tr op hen ol FA U( 20 0) Fo w le r-Gu gg en he im QFG (m g g -1) 10 2 KFG (L g -1) 3. 3 ω (KJ mol -1) -4 0. 34 1. 00 Fo r ea ch e qu ili br is ot he rm , 10 0 m g of th ad so rb en t w as ad ded t 20 0 m L of s ol ut io n t equ ili br ate f or 2 4 h ( to equ ili br iu m ) i n a ba equ ip m en t. T he in iti co nce nt ra tio ns o ad so rb at es i n w at er an bu ffe r r an ge d f ro m 1 to 5 m g L -1 a t 2 98 K a t c ons ta pH . 4-ni tr op hen ol FA U( 20 0) Fo w le r-Gu gg en he im Q FG (m g g -1) 11 0 K FG (L g -1) 3. 6 ω (KJ mol -1) -4.2 0. 39 1. 00 2, 4-di ch lo ro ph en ol FA U( 20 0) Fo w le r-Gu gg en he im QFG (m g g -1) 19 0 KFG (L g -1) 20 ω (KJ mol -1) -3.7 3. 80 1. 00 3, 4-di ch lo ro ph en ol FA U( 20 0) Fo w le r-Gu gg en he im QFG (m g g -1) 18 5 KFG (L g -1) 18 ω (KJ mol -1) -3.6 3. 33 1. 00 2-ni tr oa ni line FA U( 20 0) Fo w le r-Gu gg en he im Q FG (m g g -1) 22 0 K FG (L g -1) 13 ω (KJ mol -1) -5.7 2. 86 1. 00 4-ni tr oa ni line FA U( 20 0) Fo w le r-Gu gg en he im QFG (m g g -1) 21 2 KFG (L g -1) 5. 7 ω (KJ mol -1) 1. 21 1. 00 27 | Li te ra tu re re vi ew
28 | Cha pte r 2 -5 .4 3, 4-di ch lo ro an ili ne FA U( 20 0) Fo w le r-Gu gg en he im QFG (m g g -1) 19 0 KFG (L g -1) 31 .5 ω (KJ mol -1) -3.8 5. 98 1. 00 3, -d ich lo ro an ili ne FA U( 20 0) Fo w le r-Gu gg en he im Q FG (m g g -1) 19 2 K FG (L g -1) 34 .8 ω (KJ mol -1) -3.7 6. 68 1. 00 2, 4-di ch lo ro an ili ne FA U( 20 0) Fo w le r-Gu gg en he im QFG (m g g -1) 22 0 KFG (L g -1) 40 .4 ω (KJ mol -1) -3.7 8. 89 1. 00 2, 4-di ni tr op hen ol FA U( 20 0) Fo w le r-Gu gg en he im QFG (m g g -1) 28 0 KFG (L g -1) 13 ω (KJ mol -1) -2.7 3. 64 1. 00 2-ni tr op hen ol FA U( 20 0) Fo w le r-Gu gg en he im Q FG (m g g -1) 24 0 K FG (L g -1) 13 .4 ω (KJ mol -1) -4.2 3. 22 1. 00 Su lfa m et ho xa zo le FA U( 40 0) - QM (m g g -1) 29 6 - - - - Th e c onc ent ra tio n o f su lfam eth ox az ol e s ol uti on w as 2 02 .3 µ M . Z eo lit e: su lfam eth ox az ol e s ol uti on Su lfa m et ho xa zo le MO R(4 00 ) - QM (m g g -1) 52 - - - -
Su lfa m et ho xa zo le M FI (1 00 0) - Q M (m g g -1) 96 - - - - rat io o f 1 mg :2 m L. Su sp ens io ns o f F AU o r M OR in su lfa m et ho xa zo le so lu tio n w ere s ha ke n f or 3 0 mi n, w he re as M FI f or 2 4 h . Su lfa m et ho xa zo le FA U( 20 0) Lan gmu ir QL (m g g -1) 48 1 KL (L m g -1) 0. 89 - 42 3. 55 0. 99 5 m g ze ol ite w as d os ed in a su lfa dru g s ol ut io n ( 10 mg L -1, 50 m L in M ill ip or e w at er ). p H w as ad ju st ed us ing s ul fu ri c a ci d and so di um h yd ro xi de Su lfa th ia zo le FA U( 20 0) Lan gmu ir QL (m g g -1) 44 4 KL (L m g -1) 0. 11 - 48 .7 8 0. 99 Su lfa me ra zi ne FA U( 20 0) Lan gmu ir QL (m g g -1) 30 7 KL (L m g -1) 0. 42 - 12 8. 29 0. 99 Su lfa m et hi zo le FA U( 20 0) Lan gmu ir QL (m g g -1) 26 8 KL (L m g -1) 0. 64 - 17 0. 22 0. 99 Su lfa dim id in e FA U( 20 0) Lan gmu ir QL (m g g -1) 25 3 KL (L m g -1) 0. 75 - 18 8. 06 0. 99 2-ni tr op hen ol FA U( 20 0) Lan gmu ir QL (m g g -1) 26 7. 2 KL (L m g -1) 0. 75 3 - 19 9. 39 0. 99 10 0 m g z eo lit es w as a dd ed to 2 00 m L o f s ol ut io n w ith th e in iti al co nce nt ra tio ns o ad so rb at es i n w at er an d bu ffer ran gi ng f ro m 1 t o 50 0 m g L -1 M FI (1 80 0) Lan gmu ir Q L (m g g -1) 13 5. 7 K L (L m g -1) 0. 17 4 - 23 .5 6 0. 99 M FI (8 00 ) Lan gmu ir Q L (m g g -1) 14 7. 6 K L (L m g -1) 0. 14 8 - 21 .8 1 0. 99 M FI (2 00 ) Lan gmu ir Q L (m g g -1) 11 8. 7 K L (L m g -1) 0. 10 4 - 12 .3 3 0. 99 M FI (8 0) Lan gmu ir QL (m g g -1) 83 .9 KL (L m g -1) 0. 02 2 - 1. 85 0. 99 BE A( 98 ) Lan gmu ir QL (m g g -1) 95 .0 KL (L m g -1) 0. 02 1 - 1. 99 0. 99 BE A( 42 ) Lan gmu ir QL (m g g -1) 75 .6 KL (L m g -1) 0. 01 9 - 1. 44 0. 99 Co uma ri c a ci d FA U( 14 .5 ) Lan gmu ir QL (m g g -1) KL (L m g -1) - 9. 36 0. 97 50 m g o f z eo lit es a nd 1 0 m L 29 | Li te ra tu re re vi ew
30 | Cha pte r 2 10 8 5. 8 of aq ue ou s s ol ut io n of hy dro xy ci nn ami c ac id s w ith th e s am e i ni tia l co nce nt ra tio ns f ro m 1 0 t o 50 0 m g L -1 w er e pl ac ed i n 50 mL g las s f las k FA U( 25 ) Lan gmu ir QL (m g g -1) 68 .0 KL (L m g -1) 11 .3 - 68 8. 49 0. 95 BE A( 88 ) Lan gmu ir QL (m g g -1) 12 2. 0 KL (L m g -1) 82 - 64 65 .4 7 0. 82 Fe ru lic a cid FA U( 14 .5 ) Lan gmu ir QL (m g g -1) 13 7. 0 KL (L m g -1) 1. 33 - 17 9. 34 0. 99 FA U( 25 ) Lan gmu ir QL (m g g -1) 13 1. 6 KL (L m g -1) 1. 2 - 15 5. 67 0. 99 BE A( 88 ) Lan gmu ir QL (m g g -1) 13 8. 9 KL (L m g -1) 14 4. 0 - 11 04 5 0. 76 Ci nn am ic a ci d FA U( 25 ) Lan gmu ir QL (m g g -1) 65 .8 KL (L m g -1) 8. 44 - 50 9. 57 0. 96 BE A( 88 ) Lan gmu ir QL (m g g -1) 10 8. 7 KL (L m g -1) 15 3. 33 - 90 28 .1 8 0. 75 Ery th ro my ci n FA U( 40 0) Lan gmu ir Q L (m g g -1) 42 K L (L m g -1) 2. 1 - 86 .0 8 0. 98 Th e a ds orp tio n ex pe ri m en ts w er e m ad e up of d ua l s ol ut e, i .e . w at er an d on e o f th e s tu di ed d ru gs ov er th e z eo lite s. T he equ ili bi ur m c on cen tr ati on of e ach s ol ut e w as 0 5 m g L -1. MO R(4 00 ) Lan gmu ir Q L (m g g -1) 26 K L (L m g -1) 1. 3 - 33 .2 8 0. 99 Le vo flo xa ci n FA U( 40 0) Lan gmu ir Q L (m g g -1) 45 K L (L m g -1) 1. 4 - 61 .9 6 0. 99 MO R(4 00 ) Lan gmu ir QL (m g g -1) 27 KL (L m g -1) 0. 15 - 4. 04 0. 99 M FI (1 00 0) Lan gmu ir QL (m g g -1) 16 KL (L m g -1) 0. 10 - 1. 60 0. 99 Car ba maz ep in e FA U( 40 0) Lan gmu ir QL (m g g -1) 10 0 KL (L mg -1) 3. 1 - 29 9. 30 0. 98 MO R(4 00 ) Lan gmu ir QL (m g g -1) 32 KL (L m g -1) 0. 46 - 14 .6 4 0. 99
M FI (1 00 0) Lan gmu ir QL (m g g -1) 26 KL (L m g -1) 0. 52 - 13 .4 3 0. 99 α-end os ul fa n FA U( 34 ) Lan gmu ir QL (m g g -1) 83 3 KL (L g -1) 0. 92 3 - 0. 77 1. 00 20 0 m g z eo lit es w er e d os ed in to α -e nd os ul fa n s ol ut io n w ith co nce nt ra tio n 10 – 3 0 m g L -1 FA U( 26 ) Lan gmu ir Q L (m g g -1) 66 7 K L (L g -1) 0. 57 7 - 0. 38 1. 00 FA U( 22 ) Lan gmu ir Q L (m g g -1) 50 0 K L (L g -1) 0. 34 5 - 0. 17 1. 00 BE A( 11 0) Lan gmu ir QL (m g g -1) 79 4 KL (L g -1) 0. 49 0 - 0. 39 1. 00 BE A( 63 ) Lan gmu ir QL (m g g -1) 78 7 KL (L g -1) 0. 41 0 - 0. 32 1. 00 BE A( 36 ) Lan gmu ir Q L (m g g -1) 76 3 K L (L g -1) 0. 24 7 - 0. 19 1. 00 BE A( 33 ) Lan gmu ir Q L (m g g -1) 74 1 K L (L g -1) 0. 20 5 - 0. 15 1. 00 Tri s- 2-ch lo ro et hy l ph os ph at e (T CE P) BE A( 50 ) Lan gmu ir QL (m g g -1) 76 .6 49 KL (L µ g -1) 0. 00 78 - 0. 55 0. 96 Th e r es pec tiv e ze ol ite do sa ge w as a dd ed to a 200 mL al iq uo t o f 1 0 mg L TC EP s ol uti on . T he z eo lit es w er e do se d by v al ue s o f 0 0. 09 m m ol T CE P g -1 z eo lit e. Th e so lu tio n p H w as ad jus te d us in g HC l o r N aO H to 4 .8 . BE A( 30 0) Lan gmu ir QL (m g g -1) 10 3. 00 KL (L µ g -1) 0. 00 30 - 0. 30 0. 98 Ni co tin e BE A( 43 ) Si ps Qs (m ol g -1) 0. 00 1 Ks(L m ol -1) βs 18 73 9. 8 βs 1.14 1. 14 1. 13 10 0 mg d ry z eo lit es w ere do sed in 1 .5 ml w at er w ith an a pp ro pri at e a m ou nt o 0. 03 m ol L -1 ni co tine so lu tio n. T he eq ui libr iu m M FI (4 0) Si ps Qs (m ol g -1) 0. 00 07 Ks(L m ol -1) βs 32 5. 1 βs 0.34 35 51 .4 0 0. 20 31 | Li te ra tu re re vi ew
32 | Cha pte r 2 co nce nt ra tio ns a t 3 0 ° C w er e ac hi ev ed a fte r 1h o f st ir ri ng . Di me th yl am in e ( DM A) LT A Fr eu nd lic h K F (nm ol g -1)( L n mo l -1) n 33 4. 1 n 0.86 - 14 86 .2 7 0. 86 Ze ol ite s (~ 10 0 m g) w er e ad de d in to 40 m L gla ss v ia ls co nt ai ni ng 3 0 m L o f DM A so lu tio ns at va ry in g co nce nt ra tio ns (1 8 - 7 40 µ g L -1) FA U( 40 ) Fr eu nd lic h K F (nm ol g -1)( L n mo l -1) n 10 01 1. 3 n 1.14 - 20 26 .2 8 1. 14 M FI (4 0) Fr eu nd lic h KF (nm ol g -1)( L n mo l -1) n 24 39 .6 1 n 0.77 - 27 82 9. 15 0. 77 Me tfor m in e M FI (8 0) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 11 22 n 0.70 - 11 22 0. 70 Th e in iti al co nce nt ra tio n o f ea ch o f th e p ha rm ac eu tic al s w as 2 µ g L -1. Th e a ds orb en t co nce nt ra tio n v ar ie d be tw ee n 2 .5 a nd 1 00 0 m g L -1 MO R(2 00 ) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 63 0 n 0.60 - 63 0 0. 60 Lid oc ain e M FI (8 0) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 13 3 n 0.84 - 13 3 0. 84 MO R(2 00 ) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 50 12 n 0.55 - 50 12 0. 55 Li nco m yci ne M FI (8 0) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 23 39 n 1.18 - 23 39 1. 18 MO R(2 00 ) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 14 5 n 0.68 - 14 5 0. 68 Pa ra ce ta mo l MO R(2 00 ) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 8 n 0.70 - 8 0. 70 Ifo sf am id e M FI (8 0) Fr eu nd lic h K F (µg g -1)( L µ g -1) n 45 9 n 0.88 - 45 9 0. 88 MO R(2 00 ) Fr eu nd lic h K F (µg g -1)( L µ g -1) n 51 n 0.81 - 51 0. 88 Cy cl op ho sp ha m id e M FI (8 0) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 22 n 0.90 - 22 0. 90
MO R(2 00 ) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 13 2 n 0.82 - 13 2 0. 82 Car ba maz ep in e MO R(2 00 ) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 31 n 0.80 - 31 0. 80 Su lfa m et ho xa zo le M FI (8 0) Fr eu nd lic h K F (µg g -1)( L µ g -1) n 63 n 1.18 - 63 1. 18 MO R(2 00 ) Fr eu nd lic h K F (µg g -1)( L µ g -1) n 36 n 0.91 - 36 0. 91 Ge mf ib ro zi l M FI (8 0) Fr eu nd lic h K F (µg g -1)( L µ g -1) n 9. 20 ×1 0 -5 n 0.40 - 9. 20 *1 0 -5 0. 40 N ap ro xe n MO R(2 00 ) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 59 7 n 0.39 - 59 7 0. 39 Ph en azo n MO R(2 00 ) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 10 54 n 0.41 - 10 54 0. 41 Ke to pr of en MO R(2 00 ) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 23 0 n 0.48 - 23 0 0. 48 Cl of ib ri c a ci d MO R(2 00 ) Fr eu nd lic h KF (µg g -1)( L µ g -1) n 52 n 0.55 - 52 0. 55 Th e ad so rp tio n i so th er m e qu ati on in T abl e 2-4 w er e ex pre ss ed a s b el ow : L an gmu ir, 𝑞𝑞𝑒𝑒 = 𝑄𝑄𝐿𝐿 𝐾𝐾𝐿𝐿 𝐶𝐶𝑡𝑡 1+ 𝐾𝐾𝐿𝐿 𝐶𝐶𝑡𝑡 ; Si ps , 𝑞𝑞𝑒𝑒 = 𝐾𝐾𝑠𝑠 𝑄𝑄𝑠𝑠 𝐶𝐶𝑡𝑡 𝛽𝛽𝑠𝑠 1+ 𝐾𝐾𝑠𝑠 𝐶𝐶𝑡𝑡 𝛽𝛽𝑠𝑠 ; R ed lic h-Pe te rs on , 𝑞𝑞𝑒𝑒 = 𝐾𝐾𝑅𝑅 𝐶𝐶𝑡𝑡 1+ 𝑟𝑟𝑅𝑅 𝐶𝐶𝑡𝑡 𝛽𝛽𝑅𝑅 ; F re un 𝑞𝑞𝑒𝑒 = 𝐾𝐾𝐹𝐹 𝐶𝐶𝑒𝑒 𝑛𝑛 ; F ow ler -Gu gg en he im , 𝐾𝐾𝐹𝐹𝐹𝐹 𝐶𝐶𝑒𝑒 = 𝜃𝜃 1−𝜃𝜃 𝑒𝑒 𝑒𝑒𝑒𝑒 � 2𝜃𝜃𝜃𝜃 𝑅𝑅𝑅𝑅 �, Wh ere 𝜃𝜃 = 𝑞𝑞𝑡𝑡 . C 𝑄𝑄𝐹𝐹𝐹𝐹 e is t he e qu ili br iu m c on cen tr at io n. q e i s e qu ili br iu m ad so rp tio n c ap ac ity . Q M ma xi mu m a mo un t o f O M Ps ad so rb ed b y h ig h-si lic a z eo lites . * T he Fr eu nd lic h i so th er m co ns tan ts w er e r ec al cu lat ed b y th e i so th er m d at a g iv en in th e l ite ratu re . T he fi tti ng co nc en tr at io n ran ge w as 0 .0 1 – 70 µ g L -1. (1 ) (Go nz al ez -Ol mo s e t al ., 2 01 3) ; (2 ) (H e a nd C he ng 2 01 6) ; ( 3) (d e R id de r e t a l., 20 12 ); ( 4) (D amj an ov ic e t a l., 2 01 0) ; (5 ) (Ts ai e t al ., 2 00 6) ; ( 6) Z ha ng (2 01 4) ; ( 7) (K oub ai ss y et a l., 2 01 1) ; (8 ) ( Bl as io li e t a l., 2 01 4) ; (9 ) ( Fu kah ori e t al ., 2 01 1) ; ( 10 ) ( Re un go at e t a l., 20 07 ); (1 1) (S im on e t a l., 2 01 5) ; (1 2) (M ar al ., 2 01 2) ; ( 13 ) ( Yo nl i e t a l., 20 12 ); ( 14 ) (G rie co a nd R am ar ao 2 01 3) ; (1 5) (R ak ic e t a l., 2 01 0) ; ( 16 ) ( He a nd C he ng 20 16 ). 33 | Li te ra tu re re vi ew
High-silica zeolites were also tested for the adsorption of OMP mixtures. For example, MFI and MOR type zeolites were tested for the removal of 16 pharmaceuticals in both demineralised and surface water. When the initial concentration of each pharmaceutical
was 2 µg L-1, MOR zeolites with a Si/Al ratio of 400 either completely or considerably
removed 15 species from the mixed solution (de Ridder et al., 2012). Rossner et al. (2009) investigated the removal of a 25 OMP mixture with concentrations between 200 and 900 ng L-1 in lake water by two high-silica zeolites i.e. MOR and FAU zeolites, activated carbon
and a carbonaceous resin. Activated carbon was able to remove most of the tested compounds, while only 15 compounds were either completely or partially removed with the MOR zeolite and 3 compounds (fluoxetine, oxybenzone, and triclosan) with the FAU zeolite. It was demonstrated that effective adsorbents for the removal of a broad spectrum of OMPs from water should exhibit heterogeneity in pore size and shape.
Prediction of adsorption on high-silica zeolites at environmentally relevant concentrations The adsorption by high-silica zeolites varied with the equilibrium concentration of OMPs.
When the concentration of OMPs in the experiment was high (ranges of mg L-1), the
adsorption limit could be predicted by the adsorption isotherm models such as Langmuir and Sips (Martucci et al., 2012; Yonli et al., 2012). The estimated maximum adsorption capacity of OMPs by high-silica zeolites was then in the range of 16 to 833 mg g-1 (Table 4).
The adsorption isotherms of OMPs at environmentally realistic concentration range (µg L-1
and ng L-1) follow the Freundlich isotherm, since no concentration independent plateau is
observed from these isotherms. The maximum adsorption capacity of zeolites cannot be predicted at these concentrations (de Ridder et al., 2012; Gonzalez-Olmos et al., 2013). To compare the adsorption efficiency of OMPs in various conditions, the constants for the Freundlich isotherm model were also determined for the high concentration experiments, translating them to environmentally relevant concentrations ranging from 0.01 to 70 µg L-1.
In addition, the values of the Freundlich isotherm constant KF given with different units
were unified, since they are unit dependent. The recalculated isotherm constants are listed in Table 4, including the KF with a unit of (µg g-1)(L µg -1)n and the n value. When n was